crystal structures, polymerization, and thermochromic phase changes in urethane-substituted...
Post on 19-Feb-2017
Embed Size (px)
Crystal Structures, Polymerization, and ThermochromicPhase Changes in Urethane-Substituted Diacetylenes
Crystals with Varying Alkyl Chain LengthsHiroaki Tachibana,*,, Reiji Kumai, Noriko Hosaka, and Yoshinori Tokura,
Joint Research Center for Atom Technology, Tsukuba 305-8562, Japan, National Institute ofMaterials and Chemical Research, Tsukuba 305-8565, Japan, and Department of Applied
Physics, University of Tokyo, Tokyo 113-8656, Japan
Received July 14, 2000. Revised Manuscript Received October 16, 2000
A series of urethane-substituted diacetylene monomers (DA-mUPh) with different alkylchain length (m ) 4, 5, and 6) in side-chain substituents of (CH2)mOCONHC6H5 wassynthesized. X-ray structural analyses for the DA-mUPh single crystals show that themonomers are packed by hydrogen bonding between the urethane groups, but the arrange-ment of the diacetylene moieties depends on the alkyl chain length. The reactivity of theDA-mUPh crystals upon -irradiation is different depending whether the alkyl chain length(m) is odd or even. The difference can be explained by the distance between the neighboringcarbon atoms of the diacetylene groups. The temperature dependence of reflectance spectrafor the polydiacetylene crystals has also been investigated. The thermochromic behavior isargued in comparison with the analysis of the differential scanning calorimetry.
Diacetylenes are known to undergo solid-state polym-erization on irradiation by UV light or -rays.1-6 Twospectroscopically distinct forms, A (blue) and B (red)forms, have been observed for -conjugated polydiacety-lenes (PDA) in single crystals, Langmuir-Blodgettfilms, vacuum-deposited films, cast films, and bilayersdispersed in water. Much work has been done on thecharacterization and polymerization of various diacety-lenes derivatives. Among them, poly(ETDU) [5,7-dodec-adiyne-1,12-diol bis(ethylurethane)] is typical of thePDAs that exhibit a reversible thermochromic transitionbetween the A and the B form.7 The hydrogen bondingbetween the urethane groups plays an important rolein the reversible thermochromic behaviors, which havebeen analyzed by various measurements such as X-raydiffraction, NMR, UV-visible, IR, and Raman spectros-copy.8 Recently, photoinduced phase transitions betweenthe two forms have been also reported in one of thoseurethane-substituted PDA, a single crystal of poly-4U3[5,7-dodecadiyne-1,12-diol bis(propylurethane)].9
The alkylurethane-substituted PDAs have two kindsof alkyl chains in the side group; one is an inner alkyl
chain between PDA backbones and urethane groups,and the other one is an outer alkyl chain outside theurethane groups. Little is known on the effect of inneralkyl chain length on the structure and thermochromicbehavior of the urethane-substituted PDAs,10,11 thoughthe rather minimal effect of the outer alkyl chain lengthhas been well investigated.12
In this paper, we report the synthesis of a series ofurethane-substituted diacetylenes having side groupsof R ) (CH2)mOCONHC6H5 with various lengths ofinner alkyl chain (m ) 4, 5, 6). The effect of the alkylchain length on topochemical polymerization was in-vestigated in conjunction with the X-ray crystallo-graphic analysis of the single crystals. Thermochromicbehaviors of the derived PAD crystals were also studiedby measurements of UV-visible reflectance spectra anddifferential scanning calorimetry.
Experimental SectionUrethane-substituted diacetylenes having side groups of
R ) (CH2)mOCONHC6H5 with various lengths of alkyl chain(m ) 4, 5, 6) were synthesized as described previously (Chart1).13,14 -Bromo alcohol derivatives were protected as tBuMe2-Si (tert-butyldimethylsilyl) ethers, followed by treatment withlithium acetylide-ethylenediamine complex to give the acety-lene derivatives. After deprotection of the tBuMe2Si groupswith methanesulfonic acid, the obtained acetylene alcohol wasconverted to the urethane-substituted acetylenes by reaction
Joint Research Center for Atom Technology. National Institute of Materials and Chemical Research. University of Tokyo.(1) Wegner, G. Z. Naturforsch. 1969, 26b, 824.(2) Polydiacetylenes; Cantow, H.-J., Ed.; Springer-Verlag: Berlin,
1984.(3) Polydiacetylenes Synthesis, Structure and Electronic Properties;
Bloor, D., Chance, R. R., Eds.; Nijhoff: Dordrecht, The Netherlands,1985; Vol. 102.
(4) Tieke, B. Adv. Polym. Sci. 1985, 71, 79.(5) Schweizer, K. S. J. Chem. Phys. 1986, 85, 4181.(6) Okada, S. O.; Peng, S.; Spevak, W.; Charych, D. Acc. Chem. Res.
1997, 31, 229.(7) Chance, R. R.; Baughman, R. H.; Muller, H.; Eckhardt, C. J. J.
Chem. Phys. 1977, 67, 3616.(8) Sandman, D. J. Trends Polym. Sci. 1994, 2, 44.(9) Koshihara, S.; Tokura, Y.; Takeda, K.; Koda, T. Phys. Rev. B
1995, 52, 6265.
(10) Campbell, A. J.; Davies, C. K. L.; Batchelder, D. N. Macromol.Chem. Phys. 1998, 199, 109.
(11) Eckhardt, C. J.; Starwell, J.; Morrow, M.; Muller, H. InCrystallographically Ordered Polymer; Sandman, D. J., Ed.; ACSSymposium Series; American Chemical Society: Washington, DC,1987; Vol. 337, p 154.
(12) Koshihara, S.; Tokura, Y.; Takeda, K.; Koda, T.; Kobayashi,A. J. Chem. Phys. 1990, 92, 7581.
(13) Sandman, D. J.; Samuelson, L. A.; Velazquez, C. S. Polym.Commun. 1986, 2, 242.
(14) Kalivretenos, A.; Stille, J. K.; Hegedus, L. S. J. Org. Chem.1991, 56, 2883.
155Chem. Mater. 2001, 13, 155-158
10.1021/cm000581r CCC: $20.00 2001 American Chemical SocietyPublished on Web 12/12/2000
with phenyl isocyanate. The desired urethane-substituteddiacetylenes were obtained by oxidative coupling of theacetylenes.
Single crystals of the monomer were grown by slow evapo-ration of the ethyl acetate. The monomer crystals were sealedin Pyrex tubes under vacuum and the polymerization wascarried out by 60Co -radiation with a dose of 60 Mrad. Thecorresponding monomer and polymer of urethane-substituteddiacetylenes with phenyl group used in this study are abbrevi-ated as DA-mUPh and PDA-mUPh (m ) 4, 5, 6), respectively.
The crystallographic data were collected at 20 C on animaging plate system (Rigaku RAXSI-IV) with Mo-KR radia-tion. The structure was solved with the TEXSAN softwarepackage of the Molecular Structure Corp. and refined withOrtep-III. Other experimental details are summarized in Table1.
Polarized reflectance spectra of the PDA-mUPh crystalswere measured in the normal-incidence condition by using apremonochromatized halogen lamp. The crystals were held ata constant temperature controlled within (1 K. Differentialscanning calorimetry (DSC) measurements were performed onthe polymer samples sealed under argon in silver puns. Aheating/cooling rate of 5 K min-1 was used. Phase transitiontemperatures were determined as the maximum points on theendo- and exotherms, and the enthalpies were evaluated fromthe integrated area under the curves.
Results and DiscussionX-ray Analysis for Monomer Crystals before
Polymerization. The effect of alkyl chain length on thecrystal structure was investigated by X-ray diffractionmeasurements of single crystals of DA-mUPh. Thecrystallographic data are summarized in Table 1. Figure1 shows the crystal structure of (a) DA-4UPh, (b) DA-5UPh, and (c) DA-6UPh. DA-4UPh and DA-5UPhcrystallize in the monoclinic system. The space groupis P21/a. The regular arrangement of diacetylene groupsalong the b axis is formed by hydrogen bonding betweenthe urethane groups. DA-6UPh also crystallizes in themonoclinic form ( ) 108.7) but has a P21/n space group.The difference in the cell parameters is merely due tothe choice of the setting. The diacetylene groups stackalong the a axis, but the packing manner between thestacks is different from that of DA-4UPh and DA-5UPh,as shown in Figure 2.
From the analysis of the obtained data, we estimatedthe intermolecular distance R between reacting carbons,
Chart 1. Chemical Structures of DiacetyleneMonomers Used in This Study
Table 1. Crystal Data at 293 K for DA-mUPh (m ) 4, 5, 6)
DA-mUPh 4 5 6
space group P21/a P21/a P21/ncrystal system monoclinic monoclinic monoclinica () 11.95 12.96 5.21b () 5.11 5.14 39.76c () 19.1 19.36 7.01 (deg) 92.64 95.53 108.7V (3) 1165.1 1283.0 1376.0Z 2 2 2dcalcd (g cm-3) 1.23 1.19 1.18(Mo-KR) (cm-1) 0.83 0.80 0.78F(000) 432 464 496no. of reflections 1357 1437 1132no. of variables 144 153 162R 0.064 0.060 0.076Rw 0.066 0.078 0.074
Figure 1. Crystal structure of (a) DA-4UPh, (b) DA-5UPh,and (c) DA-6UPh.
156 Chem. Mater., Vol. 13, No. 1, 2001 Tachibana et al.
- the stacking distance d between neighboring diacetylenemoieties along the stacking axis, and the inclinationangle between the diacetylene rod and the stackingaxis. The solid-state polymerization of diacetylenes incrystal is known to critically depend on the above threeparameters.15,16 The ideal criteria (R, d, and ) for thepolymerization is
observed at 1.96 eV. The peak at its higher energycorresponds to vibronic side bands associated with thedouble-bond stretching of the conjugated backbone.Upon heating, the crystals undergo the phase transitioninto the B form and the peak energy shifts to 2.3 eV, inagreement with the behavior reported in the litera-ture.23 The critical temperature for the A-to-B transitionis in the range of 460-470 K. The B form did notcompletely revert to the initial A form even when cooledto room temperature (300 K).
Figure 4 shows temperature dependence of reflectancespectra (polarized parallel to the polymer backbone) forthe PDA-6UPh crystals. An intense peak due to thelowest exciton of the B form is observed around 2.4 eV,in addition to the weak exciton peak due to the A formaround 2 eV. This indicates that the two forms are bothcontained in the PDA-6UPh crystal as polymerized atroom temperature. Upon heating, the weak exciton peakd